LMucko/crystallography-open-database huggingface dataset:
The temperature dependence of the cation distribution in magnesioferrite (MgFe2O4) from powder XRD structural refinements and Mossbauer spectroscopy batch 2, anneal T = 450 C using the two step method
O'Neill H St C; Annersten, H.; Virgo, D.; American Mineralogist 77 (1992) 725–740; doi:

data_9001469
_publ_section_title
;
 The temperature dependence of the cation distribution in magnesioferrite
 (MgFe2O4) from powder XRD structural refinements and Mossbauer spectroscopy
 batch 2, anneal T = 450 C using the two step method
;
_journal_name_full               'American Mineralogist'
_journal_page_first              725
_journal_page_last               740
_journal_volume                  77
_journal_year                    1992
_chemical_formula_sum            'Fe2 Mg O4'
_chemical_name_mineral           Magnesioferrite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.3806
_cell_length_b                   8.3806
_cell_length_c                   8.3806
_cell_formula_units_Z            8
_cell_volume                     588.607
_database_code_amcsd             0001507
_exptl_crystal_density_diffrn    4.514
_exptl_crystal_thermal_history   'anneal T = 450 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Mg Fe2) O4'
_cod_database_code               9001469
The temperature dependence of the cation distribution in magnesioferrite (MgFe2O4) from powder XRD structural refinements and Mossbauer spectroscopy batch 1, anneal T = 500 C using the two step method
O'Neill H St C; Annersten, H.; Virgo, D.; American Mineralogist 77 (1992) 725–740; doi:

data_9001470
_publ_section_title
;
 The temperature dependence of the cation distribution in magnesioferrite
 (MgFe2O4) from powder XRD structural refinements and Mossbauer spectroscopy
 batch 1, anneal T = 500 C using the two step method
;
_journal_name_full               'American Mineralogist'
_journal_page_first              725
_journal_page_last               740
_journal_volume                  77
_journal_year                    1992
_chemical_formula_sum            'Fe2 Mg1.001 O4'
_chemical_name_mineral           Magnesioferrite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.3827
_cell_length_b                   8.3827
_cell_length_c                   8.3827
_cell_formula_units_Z            8
_cell_volume                     589.049
_database_code_amcsd             0001508
_exptl_crystal_density_diffrn    4.511
_exptl_crystal_thermal_history   'anneal T = 500 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Mg1.001 Fe2 O4'
_cod_database_code               9001470
The temperature dependence of the cation distribution in magnesioferrite (MgFe2O4) from powder XRD structural refinements and Mossbauer spectroscopy batch 2, anneal T = 500 C using the two step method
O'Neill H St C; Annersten, H.; Virgo, D.; American Mineralogist 77 (1992) 725–740; doi:

data_9001471
_publ_section_title
;
 The temperature dependence of the cation distribution in magnesioferrite
 (MgFe2O4) from powder XRD structural refinements and Mossbauer spectroscopy
 batch 2, anneal T = 500 C using the two step method
;
_journal_name_full               'American Mineralogist'
_journal_page_first              725
_journal_page_last               740
_journal_volume                  77
_journal_year                    1992
_chemical_formula_sum            'Fe2 Mg O4'
_chemical_name_mineral           Magnesioferrite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.3827
_cell_length_b                   8.3827
_cell_length_c                   8.3827
_cell_formula_units_Z            8
_cell_volume                     589.049
_database_code_amcsd             0001509
_exptl_crystal_density_diffrn    4.510
_exptl_crystal_thermal_history   'anneal T = 500 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Mg Fe2) O4'
_cod_database_code               9001471
The temperature dependence of the cation distribution in magnesioferrite (MgFe2O4) from powder XRD structural refinements and Mossbauer spectroscopy batch 2, anneal T = 550 C using the two step method
O'Neill H St C; Annersten, H.; Virgo, D.; American Mineralogist 77 (1992) 725–740; doi:

data_9001472
_publ_section_title
;
 The temperature dependence of the cation distribution in magnesioferrite
 (MgFe2O4) from powder XRD structural refinements and Mossbauer spectroscopy
 batch 2, anneal T = 550 C using the two step method
;
_journal_name_full               'American Mineralogist'
_journal_page_first              725
_journal_page_last               740
_journal_volume                  77
_journal_year                    1992
_chemical_formula_sum            'Fe2 Mg O4'
_chemical_name_mineral           Magnesioferrite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.3845
_cell_length_b                   8.3845
_cell_length_c                   8.3845
_cell_formula_units_Z            8
_cell_volume                     589.429
_database_code_amcsd             0001510
_exptl_crystal_density_diffrn    4.507
_exptl_crystal_thermal_history   'anneal T = 550 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Mg Fe2) O4'
_cod_database_code               9001472
The temperature dependence of the cation distribution in magnesioferrite (MgFe2O4) from powder XRD structural refinements and Mossbauer spectroscopy batch 2, anneal T = 600 C using the two step method
O'Neill H St C; Annersten, H.; Virgo, D.; American Mineralogist 77 (1992) 725–740; doi:

data_9001473
_publ_section_title
;
 The temperature dependence of the cation distribution in magnesioferrite
 (MgFe2O4) from powder XRD structural refinements and Mossbauer spectroscopy
 batch 2, anneal T = 600 C using the two step method
;
_journal_name_full               'American Mineralogist'
_journal_page_first              725
_journal_page_last               740
_journal_volume                  77
_journal_year                    1992
_chemical_formula_sum            'Fe2 Mg O4'
_chemical_name_mineral           Magnesioferrite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.3863
_cell_length_b                   8.3863
_cell_length_c                   8.3863
_cell_formula_units_Z            8
_cell_volume                     589.809
_database_code_amcsd             0001511
_exptl_crystal_density_diffrn    4.505
_exptl_crystal_thermal_history   'anneal T = 600 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Mg Fe2) O4'
_cod_database_code               9001473
The temperature dependence of the cation distribution in magnesioferrite (MgFe2O4) from powder XRD structural refinements and Mossbauer spectroscopy batch 1, anneal T = 650 C using the two step method
O'Neill H St C; Annersten, H.; Virgo, D.; American Mineralogist 77 (1992) 725–740; doi:

data_9001474
_publ_section_title
;
 The temperature dependence of the cation distribution in magnesioferrite
 (MgFe2O4) from powder XRD structural refinements and Mossbauer spectroscopy
 batch 1, anneal T = 650 C using the two step method
;
_journal_name_full               'American Mineralogist'
_journal_page_first              725
_journal_page_last               740
_journal_volume                  77
_journal_year                    1992
_chemical_formula_sum            'Fe2 Mg O4'
_chemical_name_mineral           Magnesioferrite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.3883
_cell_length_b                   8.3883
_cell_length_c                   8.3883
_cell_formula_units_Z            8
_cell_volume                     590.231
_database_code_amcsd             0001512
_exptl_crystal_density_diffrn    4.501
_exptl_crystal_thermal_history   'anneal T = 650 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Mg Fe2) O4'
_cod_database_code               9001474
The temperature dependence of the cation distribution in magnesioferrite (MgFe2O4) from powder XRD structural refinements and Mossbauer spectroscopy batch 2, anneal T = 650 C using the two step method
O'Neill H St C; Annersten, H.; Virgo, D.; American Mineralogist 77 (1992) 725–740; doi:

data_9001475
_publ_section_title
;
 The temperature dependence of the cation distribution in magnesioferrite
 (MgFe2O4) from powder XRD structural refinements and Mossbauer spectroscopy
 batch 2, anneal T = 650 C using the two step method
;
_journal_name_full               'American Mineralogist'
_journal_page_first              725
_journal_page_last               740
_journal_volume                  77
_journal_year                    1992
_chemical_formula_sum            'Fe2 Mg O4'
_chemical_name_mineral           Magnesioferrite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.3883
_cell_length_b                   8.3883
_cell_length_c                   8.3883
_cell_formula_units_Z            8
_cell_volume                     590.231
_database_code_amcsd             0001513
_exptl_crystal_density_diffrn    4.501
_exptl_crystal_thermal_history   'anneal T = 650 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Mg Fe2) O4'
_cod_database_code               9001475
_cod_duplicate_entry 9001474
The temperature dependence of the cation distribution in magnesioferrite (MgFe2O4) from powder XRD structural refinements and Mossbauer spectroscopy batch 2, anneal T = 700 C using the two step method
O'Neill H St C; Annersten, H.; Virgo, D.; American Mineralogist 77 (1992) 725–740; doi:

data_9001476
_publ_section_title
;
 The temperature dependence of the cation distribution in magnesioferrite
 (MgFe2O4) from powder XRD structural refinements and Mossbauer spectroscopy
 batch 2, anneal T = 700 C using the two step method
;
_journal_name_full               'American Mineralogist'
_journal_page_first              725
_journal_page_last               740
_journal_volume                  77
_journal_year                    1992
_chemical_formula_sum            'Fe2 Mg O4'
_chemical_name_mineral           Magnesioferrite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.3899
_cell_length_b                   8.3899
_cell_length_c                   8.3899
_cell_formula_units_Z            8
_cell_volume                     590.569
_database_code_amcsd             0001514
_exptl_crystal_density_diffrn    4.499
_exptl_crystal_thermal_history   'anneal T = 700 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Mg Fe2) O4'
_cod_database_code               9001476
The temperature dependence of the cation distribution in magnesioferrite (MgFe2O4) from powder XRD structural refinements and Mossbauer spectroscopy batch 1, anneal T = 750 C using the two step method
O'Neill H St C; Annersten, H.; Virgo, D.; American Mineralogist 77 (1992) 725–740; doi:

data_9001477
_publ_section_title
;
 The temperature dependence of the cation distribution in magnesioferrite
 (MgFe2O4) from powder XRD structural refinements and Mossbauer spectroscopy
 batch 1, anneal T = 750 C using the two step method
;
_journal_name_full               'American Mineralogist'
_journal_page_first              725
_journal_page_last               740
_journal_volume                  77
_journal_year                    1992
_chemical_formula_sum            'Fe2 Mg O4'
_chemical_name_mineral           Magnesioferrite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.3914
_cell_length_b                   8.3914
_cell_length_c                   8.3914
_cell_formula_units_Z            8
_cell_volume                     590.885
_database_code_amcsd             0001515
_exptl_crystal_density_diffrn    4.496
_exptl_crystal_thermal_history   'anneal T = 750 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Mg Fe2) O4'
_cod_database_code               9001477
The temperature dependence of the cation distribution in magnesioferrite (MgFe2O4) from powder XRD structural refinements and Mossbauer spectroscopy batch 2, anneal T = 750 C using the two step method
O'Neill H St C; Annersten, H.; Virgo, D.; American Mineralogist 77 (1992) 725–740; doi:

data_9001478
_publ_section_title
;
 The temperature dependence of the cation distribution in magnesioferrite
 (MgFe2O4) from powder XRD structural refinements and Mossbauer spectroscopy
 batch 2, anneal T = 750 C using the two step method
;
_journal_name_full               'American Mineralogist'
_journal_page_first              725
_journal_page_last               740
_journal_volume                  77
_journal_year                    1992
_chemical_formula_sum            'Fe2 Mg O4'
_chemical_name_mineral           Magnesioferrite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.3914
_cell_length_b                   8.3914
_cell_length_c                   8.3914
_cell_formula_units_Z            8
_cell_volume                     590.885
_database_code_amcsd             0001516
_exptl_crystal_density_diffrn    4.496
_exptl_crystal_thermal_history   'anneal T = 750 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Mg Fe2) O4'
_cod_database_code               9001478
_cod_duplicate_entry 9001477
The temperature dependence of the cation distribution in magnesioferrite (MgFe2O4) from powder XRD structural refinements and Mossbauer spectroscopy batch 2, anneal T = 800 C using the two step method
O'Neill H St C; Annersten, H.; Virgo, D.; American Mineralogist 77 (1992) 725–740; doi:

data_9001479
_publ_section_title
;
 The temperature dependence of the cation distribution in magnesioferrite
 (MgFe2O4) from powder XRD structural refinements and Mossbauer spectroscopy
 batch 2, anneal T = 800 C using the two step method
;
_journal_name_full               'American Mineralogist'
_journal_page_first              725
_journal_page_last               740
_journal_volume                  77
_journal_year                    1992
_chemical_formula_sum            'Fe2 Mg O4'
_chemical_name_mineral           Magnesioferrite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.3934
_cell_length_b                   8.3934
_cell_length_c                   8.3934
_cell_formula_units_Z            8
_cell_volume                     591.308
_database_code_amcsd             0001517
_exptl_crystal_density_diffrn    4.493
_exptl_crystal_thermal_history   'anneal T = 800 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Mg Fe2) O4'
_cod_database_code               9001479
The temperature dependence of the cation distribution in magnesioferrite (MgFe2O4) from powder XRD structural refinements and Mossbauer spectroscopy batch 2, anneal T = 850 C using the two step method
O'Neill H St C; Annersten, H.; Virgo, D.; American Mineralogist 77 (1992) 725–740; doi:

data_9001480
_publ_section_title
;
 The temperature dependence of the cation distribution in magnesioferrite
 (MgFe2O4) from powder XRD structural refinements and Mossbauer spectroscopy
 batch 2, anneal T = 850 C using the two step method
;
_journal_name_full               'American Mineralogist'
_journal_page_first              725
_journal_page_last               740
_journal_volume                  77
_journal_year                    1992
_chemical_formula_sum            'Fe2 Mg O4'
_chemical_name_mineral           Magnesioferrite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.3946
_cell_length_b                   8.3946
_cell_length_c                   8.3946
_cell_formula_units_Z            8
_cell_volume                     591.562
_database_code_amcsd             0001518
_exptl_crystal_density_diffrn    4.491
_exptl_crystal_thermal_history   'anneal T = 850 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Mg Fe2) O4'
_cod_database_code               9001480
_cod_duplicate_entry 9001458
The temperature dependence of the cation distribution in magnesioferrite (MgFe2O4) from powder XRD structural refinements and Mossbauer spectroscopy batch 1, anneal T = 900 C using the two step method
O'Neill H St C; Annersten, H.; Virgo, D.; American Mineralogist 77 (1992) 725–740; doi:

data_9001481
_publ_section_title
;
 The temperature dependence of the cation distribution in magnesioferrite
 (MgFe2O4) from powder XRD structural refinements and Mossbauer spectroscopy
 batch 1, anneal T = 900 C using the two step method
;
_journal_name_full               'American Mineralogist'
_journal_page_first              725
_journal_page_last               740
_journal_volume                  77
_journal_year                    1992
_chemical_formula_sum            'Fe2 Mg O4'
_chemical_name_mineral           Magnesioferrite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.3959
_cell_length_b                   8.3959
_cell_length_c                   8.3959
_cell_formula_units_Z            8
_cell_volume                     591.837
_database_code_amcsd             0001519
_exptl_crystal_density_diffrn    4.489
_exptl_crystal_thermal_history   'anneal T = 900 C'
_cod_original_cell_volume        591.836
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Mg Fe2) O4'
_cod_database_code               9001481
The temperature dependence of the cation distribution in magnesioferrite (MgFe2O4) from powder XRD structural refinements and Mossbauer spectroscopy batch 2, anneal T = 900 C using the two step method
O'Neill H St C; Annersten, H.; Virgo, D.; American Mineralogist 77 (1992) 725–740; doi:

data_9001482
_publ_section_title
;
 The temperature dependence of the cation distribution in magnesioferrite
 (MgFe2O4) from powder XRD structural refinements and Mossbauer spectroscopy
 batch 2, anneal T = 900 C using the two step method
;
_journal_name_full               'American Mineralogist'
_journal_page_first              725
_journal_page_last               740
_journal_volume                  77
_journal_year                    1992
_chemical_formula_sum            'Fe2 Mg O4'
_chemical_name_mineral           Magnesioferrite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.3959
_cell_length_b                   8.3959
_cell_length_c                   8.3959
_cell_formula_units_Z            8
_cell_volume                     591.837
_database_code_amcsd             0001520
_exptl_crystal_density_diffrn    4.489
_exptl_crystal_thermal_history   'anneal T = 900 C'
_cod_original_cell_volume        591.836
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Mg Fe2) O4'
_cod_database_code               9001482
The temperature dependence of the cation distribution in magnesioferrite (MgFe2O4) from powder XRD structural refinements and Mossbauer spectroscopy batch 1, anneal T = 950 C using the two step method
O'Neill H St C; Annersten, H.; Virgo, D.; American Mineralogist 77 (1992) 725–740; doi:

data_9001483
_publ_section_title
;
 The temperature dependence of the cation distribution in magnesioferrite
 (MgFe2O4) from powder XRD structural refinements and Mossbauer spectroscopy
 batch 1, anneal T = 950 C using the two step method
;
_journal_name_full               'American Mineralogist'
_journal_page_first              725
_journal_page_last               740
_journal_volume                  77
_journal_year                    1992
_chemical_formula_sum            'Fe2 Mg O4'
_chemical_name_mineral           Magnesioferrite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.3970
_cell_length_b                   8.3970
_cell_length_c                   8.3970
_cell_formula_units_Z            8
_cell_volume                     592.069
_database_code_amcsd             0001521
_exptl_crystal_density_diffrn    4.487
_exptl_crystal_thermal_history   'anneal T = 950 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Mg Fe2) O4'
_cod_database_code               9001483